Thickness (mm) AS 3706.1 1.6 2.0 – Note 1 test shall be completed using Class 170 bitumen as per AS 2008. The sample of bitumen shall be – reheated only once. Note 2 results are to be reported for both fabric directions. Test specimens are to be exposed for a period – of 500 ± 50 hours with a total exposure of 630 KJ/m2. Note 3 geotextile fabric shall be dry conditioned prior to testing. – A roll of geotextile fabric shall: Geotextile Roll Be rolled on to a PVC tube Be evenly wound on to the tube to create square ends with the roll varying no more than 40mm in rolled width Be within 50mm of the ordered width for the full length of the roll Not be shorter than the ordered length and be no more than 1m longer. When stored Geotextile fabric be: Storage wrapped with a waterproof opaque material including the ends of rolls stored in a shed away from direct sunlight and rain kept off the ground and away from any source of moisture. Rolls of Geotextile fabric shall show the manufacturer’s name, batch Labelling number and date of manufacture. Geotextile fabric shall be used within 2 years of the date of manufacture. Age The Contractor test the geotextile fabric for conformance to the Compliance properties in Table 511.15 and at the testing frequency shown in Testing Specification 201 QUALITY SYSTEMS. Testing shall be undertaken in a laboratory accredited by NATA or a laboratory accredited by a body that is signatory to the ILAC Mutual Recognition Agreement. 511.21 511.80 NOT USED – AS AND HANDOVER REQUIREMENTS 511.81 511.90 NOT USED – CONTRACT SPECIFIC REQUIREMENTS 511.91 511.99 NOT USED –
Thickness (mm) AS 3706.1 1.6 – 2.0 Note 1 – test shall be completed using Class 170 bitumen as per AS 2008. The sample of bitumen shall be reheated only once. Note 2 – results are to be reported for both fabric directions. Test specimens are to be exposed for a period of 500 ± 50 hours with a total exposure of 630 KJ/m2. Note 3 – geotextile fabric shall be dry conditioned prior to testing. A roll of geotextile fabric shall: Geotextile Roll Be rolled on to a PVC tube Be evenly wound on to the tube to create square ends with the roll varying no more than 40mm in rolled width Be within 50mm of the ordered width for the full length of the roll Not be shorter than the ordered length and be no more than 1m longer. When stored Geotextile fabric be: Storage wrapped with a waterproof opaque material including the ends of rolls stored in a shed away from direct sunlight and rain kept off the ground and away from any source of moisture. Rolls of Geotextile fabric shall show the manufacturer’s name, batch number and date of manufacture. Labelling Geotextile fabric shall be used within 2 years of the date of manufacture. Age The Contractor test the geotextile fabric for conformance to the properties in Table 511.15 and at the testing frequency shown in Specification 201 QUALITY SYSTEMS. Testing shall be undertaken in a laboratory accredited by NATA or a laboratory accredited by a body that is signatory to the ILAC Mutual Recognition Agreement. Compliance Testing 511.21 – 511.80 NOT USED AS AND HANDOVER REQUIREMENTS 511.81 – 511.90 NOT USED CONTRACT SPECIFIC REQUIREMENTS 511.91 – 511.99 NOT USED
Specification%20511%20Materials%20for%20Bituminous%20Treatments%2023%20May%202017.RCN-D17^23399745.DOCX